1 14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation. Calculate the resulting strain. This problem calls for us to calculate the elastic strain that results for an aluminum specimen stressed in tension. The cross-sectional area is just (10 mm) (12.7 mm) 127 mm 2 ( m in. 2 ); also, the elastic modulus for Al is given in Table 6.1 as 69 GPa (or N/m 2 ). Combining Equations 6.1 and 6.5 and solving for the strain yields E F A 0 E 35,500 N ( m 2 )( N/m ) Question 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm (0.8 in.) on an edge is pulled in tension with a load of 89,000 N (20,000 lb f ), and experiences an elongation of 0.10 mm ( in.). Assuming that the deformation is entirely elastic, calculate the elastic modulus of the steel. This problem asks us to compute the elastic modulus of steel. For a square cross-section, A 0 b 2 0, where b 0 is the edge length. Combining Equations 6.1, 6.2, and 6.5 and solving for E, leads to E F A 0 l l 0 Fl 0 b 0 2 l (89,000 N)( m) ( m) 2 ( m) N/m GPa ( psi)
2 Question 6.7: For a bronze alloy, the stress at which plastic deformation begins is 275 MPa (40,000 psi), and the modulus of elasticity is 115 GPa ( psi). (a) What is the maximum load that may be applied to a specimen with a cross-sectional area of 325 mm 2 (0.5 in. 2 ) without plastic deformation? (b) If the original specimen length is 115 mm (4.5 in.), what is the maximum length to which it may be stretched without causing plastic deformation? (a) This portion of the problem calls for a determination of the maximum load that can be applied without plastic deformation (F y ). Taking the yield strength to be 275 MPa, and employment of Equation 6.1 leads to F y y A 0 ( N/m 2 )( m 2 ) 89,375 N (20,000 lb f ) (b) The maximum length to which the sample may be deformed without plastic deformation is determined from Equations 6.2 and 6.5 as l i l 0 1 E 275 MPa (115 mm) mm (4.51 in.) MPa Question 6.13: In Section 2.6 it was noted that the net bonding energy E N between two isolated positive and negative ions is a function of interionic distance r as follows: E N A r B r n (6.25) where A, B, and n are constants for the particular ion pair. Equation 6.25 is also valid for the bonding energy between adjacent ions in solid materials. The modulus of elasticity E is proportional to the slope of the interionic force separation curve at the equilibrium interionic separation; that is,
3 E df dr r o Derive an expression for the dependence of the modulus of elasticity on these A, B, and n parameters (for the two-ion system) using the following procedure: 1. Establish a relationship for the force F as a function of r, realizing that F de N dr 2. Now take the derivative df/dr. 3. Develop an expression for r 0, the equilibrium separation. Since r 0 corresponds to the value of r at the minimum of the E N -versus-r curve (Figure 2.8b), take the derivative de N /dr, set it equal to zero, and solve for r, which corresponds to r Finally, substitute this expression for r 0 into the relationship obtained by taking df/dr. This problem asks that we derive an expression for the dependence of the modulus of elasticity, E, on the parameters A, B, and n in Equation It is first necessary to take de N /dr in order to obtain an expression for the force F; this is accomplished as follows: F de N dr d A r + dr d B r n dr A r 2 nb r (n 1) The second step is to set this de N /dr expression equal to zero and then solve for r ( r 0 ). The algebra for this procedure is carried out in Problem 2.14, with the result that r 0 A 1/(1 n) nb Next it becomes necessary to take the derivative of the force (df/dr), which is accomplished as follows:
4 df dr d A r 2 + dr d nb r (n 1) dr 2 A (n)(n 1)B + r 3 r (n 2) Now, substitution of the above expression for r 0 into this equation yields df dr r 0 2A A 3/(1 n) nb + (n)(n 1) B A (n 2)/(1 n) nb which is the expression to which the modulus of elasticity is proportional. Question 6.14: Using the solution to Problem 6.13, rank the magnitudes of the moduli of elasticity for the following hypothetical X, Y, and Z materials from the greatest to the least. The appropriate A, B, and n parameters (Equation 6.25) for these three materials are tabulated below; they yield E N in units of electron volts and r in nanometers: Material A B n X Y Z This problem asks that we rank the magnitudes of the moduli of elasticity of the three hypothetical metals X, Y, and Z. From Problem 6.13, it was shown for materials in which the bonding energy is dependent on the interatomic distance r according to Equation 6.25, that the modulus of elasticity E is proportional to 2A E A 3/(1 n) nb + (n)(n 1) B A (n 2)/(1 n) nb For metal X, A 2.5, B , and n 8. Therefore,
5 (2)(2.5) E 3/(1 8) 2.5 (8)( ) + (8)(8 1)( ) (8 2)/(1 8) 2.5 (8)( ) 1097 For metal Y, A 2.3, B , and n Hence E (2)(2.3) 3/(1 10.5) 2.3 (10.5) ( ) + (10.5)(10.5 1)( ) (10.5 2)/(1 10.5) 2.3 (10.5) ( ) 551 And, for metal Z, A 3.0, B , and n 9. Thus E (2)(3.0) 3/(1 9) 3.0 (9)( ) + (9)(9 1)( ) (9 2)/(1 9) 3.0 (9)( ) 1024 Therefore, metal X has the highest modulus of elasticity. Question 15: A cylindrical specimen of aluminum having a diameter of 19 mm (0.75 in.) and length of 200 mm (8.0 in.) is deformed elastically in tension with a force of 48,800 N (11,000 lb f ). Using the data contained in Table 6.1, determine the following: (a) The amount by which this specimen will elongate in the direction of the applied stress. (b) The change in diameter of the specimen. Will the diameter increase or decrease? (a) We are asked, in this portion of the problem, to determine the elongation of a cylindrical specimen of aluminum. Combining Equations 6.1, 6.2, and 6.5, leads to
6 E F d 0 2 E l l 0 4 Or, solving for l (and realizing that E 69 GPa, Table 6.1), yields l 4Fl 0 d 0 2 E (4)(48,800 N)( m) ( )( m) 2 ( N/m 2 ) m 0.50 mm (0.02 in.) (b) We are now called upon to determine the change in diameter, d. Using Equation 6.8 x z d / d 0 l /l 0 From Table 6.1, for aluminum, Now, solving the above expression for d yields d ld 0 l 0 (0.33)(0.50 mm)(19 mm) 200 mm mm ( in.) The diameter will decrease. Question 6.20: A brass alloy is known to have a yield strength of 275 MPa (40,000 psi), a tensile strength of 380 MPa (55,000 psi), and an elastic modulus of 103 GPa ( psi). A cylindrical specimen of this alloy 12.7 mm (0.50 in.) in diameter and 250 mm (10.0 in.) long is stressed in tension and found to elongate 7.6 mm (0.30 in.). On the basis of the information given, is it possible to compute the magnitude of the load that is necessary to produce this change in length? If so, calculate the load. If not, explain why.
7 We are asked to ascertain whether or not it is possible to compute, for brass, the magnitude of the load necessary to produce an elongation of 7.6 mm (0.30 in.). It is first necessary to compute the strain at yielding from the yield strength and the elastic modulus, and then the strain experienced by the test specimen. Then, if (test) < (yield) deformation is elastic, and the load may be computed using Equations 6.1 and 6.5. However, if (test) > (yield) computation of the load is not possible inasmuch as deformation is plastic and we have neither a stress-strain plot nor a mathematical expression relating plastic stress and strain. We compute these two strain values as (test) l l mm 250 mm 0.03 and (yield) y E 275 MPa MPa Therefore, computation of the load is not possible since (test) > (yield). Question 6.22: Consider the brass alloy for which the stress-strain behavior is shown in Figure A cylindrical specimen of this material 6 mm (0.24 in.) in diameter and 50 mm (2 in.) long is pulled in tension with a force of 5000 N (1125 lb f ). If it is known that this alloy has a Poisson's ratio of 0.30, compute: (a) the specimen elongation, and (b) the reduction in specimen diameter. (a) This portion of the problem asks that we compute the elongation of the brass specimen. The first calculation necessary is that of the applied stress using Equation 6.1, as F A 0 F d N m N/m MPa (25,000 psi) 2 2
8 From the stress-strain plot in Figure 6.12, this stress corresponds to a strain of about From the definition of strain, Equation 6.2 l l 0 ( )(50 mm) 0.10 mm ( in.) (b) In order to determine the reduction in diameter d, it is necessary to use Equation 6.8 and the definition of lateral strain (i.e., x d/d 0 ) as follows d d 0 x d 0 z (6 mm)(0.30)( ) mm ( in.) Question 6.27: A load of 85,000 N (19,100 lb f ) is applied to a cylindrical specimen of a steel alloy (displaying the stress strain behavior shown in Figure 6.21) that has a cross-sectional diameter of 15 mm (0.59 in.). (a) Will the specimen experience elastic and/or plastic deformation? Why? (b) If the original specimen length is 250 mm (10 in.), how much will it increase in length when this load is applied? This problem asks us to determine the deformation characteristics of a steel specimen, the stress-strain behavior for which is shown in Figure (a) In order to ascertain whether the deformation is elastic or plastic, we must first compute the stress, then locate it on the stress-strain curve, and, finally, note whether this point is on the elastic or plastic region. Thus, from Equation 6.1 F A 0 85, 000 N m N/m MPa (69,900 psi) 2 The 481 MPa point is beyond the linear portion of the curve, and, therefore, the deformation will be both elastic and plastic. (b) This portion of the problem asks us to compute the increase in specimen length. From the stress-strain curve, the strain at 481 MPa is approximately Thus, from Equation 6.2
9 l l 0 (0.0135)(250 mm) 3.4 mm (0.135 in.) Question 6.28: A bar of a steel alloy that exhibits the stress-strain behavior shown in Figure 6.21 is subjected to a tensile load; the specimen is 300 mm (12 in.) long, and of square cross section 4.5 mm (0.175 in.) on a side. (a) Compute the magnitude of the load necessary to produce an elongation of 0.45 mm (0.018 in.). (b) What will be the deformation after the load has been released? (a) We are asked to compute the magnitude of the load necessary to produce an elongation of 0.45 mm for the steel displaying the stress-strain behavior shown in Figure First, calculate the strain, and then the corresponding stress from the plot. l l mm 300 mm This is near the end of the elastic region; from the inset of Figure 6.21, this corresponds to a stress of about 300 MPa (43,500 psi). Now, from Equation 6.1 F A 0 b 2 in which b is the cross-section side length. Thus, F ( N/m 2 )( m) N (1366 lb f ) (b) After the load is released there will be no deformation since the material was strained only elastically.
10 Question 6.29: A cylindrical specimen of aluminum having a diameter of in. (12.8 mm) and a gauge length of in. ( mm) is pulled in tension. Use the load elongation characteristics tabulated below to complete parts (a) through (f). Load Length N lb f mm in ,330 1, ,100 3, ,100 5, ,400 6, ,400 7, ,400 8, ,300 9, ,800 10, ,200 10, ,300 10, ,500 10, ,100 10, ,800 10, ,600 9, ,400 8, Fracture (a) Plot the data as engineering stress versus engineering strain. (b) Compute the modulus of elasticity. (c) Determine the yield strength at a strain offset of (d) Determine the tensile strength of this alloy. (e) What is the approximate ductility, in percent elongation? (f) Compute the modulus of resilience. This problem calls for us to make a stress-strain plot for aluminum, given its tensile load-length data, and then to determine some of its mechanical characteristics.
11 (a) The data are plotted below on two plots: the first corresponds to the entire stress-strain curve, while for the second, the curve extends to just beyond the elastic region of deformation. (b) The elastic modulus is the slope in the linear elastic region (Equation 6.10) as E 200 MPa 0 MPa MPa 62.5 GPa ( psi)
12 (c) For the yield strength, the strain offset line is drawn dashed. It intersects the stress-strain curve at approximately 285 MPa (41,000 psi ). (d) The tensile strength is approximately 370 MPa (54,000 psi), corresponding to the maximum stress on the complete stress-strain plot. (e) The ductility, in percent elongation, is just the plastic strain at fracture, multiplied by one-hundred. The total fracture strain at fracture is 0.165; subtracting out the elastic strain (which is about 0.005) leaves a plastic strain of Thus, the ductility is about 16%EL. (f) From Equation 6.14, the modulus of resilience is just U r y 2 2E which, using data computed above gives a value of U r (285 MPa) 2 (2)( MPa) 0.65 MN/m N/m J/m 3 (93.8 in.- lb f /in. 3 ) Question 6.40: Demonstrate that Equation 6.16, the expression defining true strain, may also be represented by T ln when specimen volume remains constant during deformation. Which of these two expressions is more valid during necking? Why? This problem asks us to demonstrate that true strain may also be represented by A 0 A i T ln A 0 A i Rearrangement of Equation 6.17 leads to
13 l i l 0 A 0 A i Thus, Equation 6.16 takes the form T ln l i l 0 ln A 0 A i The expression T ln A 0 A i is more valid during necking because A i is taken as the area of the neck. Question 6.44: The following true stresses produce the corresponding true plastic strains for a brass alloy: True Stress (psi) True Strain 50, , What true stress is necessary to produce a true plastic strain of 0.25? For this problem, we are given two values of T and T, from which we are asked to calculate the true stress which produces a true plastic strain of Employing Equation 6.19, we may set up two simultaneous equations with two unknowns (the unknowns being K and n), as log (50,000 psi) log K + n log (0.10) log (60,000 psi) log K + n log (0.20) Solving for n from these two expressions yields n log (50,000) log (60,000) log (0.10) log (0.20) and for K
14 log K 4.96 or K ,623 psi Thus, for T 0.25 T K ( T ) n (91,623 psi)(0.25) ,700 psi (440 MPa) Question 6.46: Find the toughness (or energy to cause fracture) for a metal that experiences both elastic and plastic deformation. Assume Equation 6.5 for elastic deformation, that the modulus of elasticity is 172 GPa ( psi), and that elastic deformation terminates at a strain of For plastic deformation, assume that the relationship between stress and strain is described by Equation 6.19, in which the values for K and n are 6900 MPa ( psi) and 0.30, respectively. Furthermore, plastic deformation occurs between strain values of 0.01 and 0.75, at which point fracture occurs. This problem calls for us to compute the toughness (or energy to cause fracture). The easiest way to do this is to integrate both elastic and plastic regions, and then add them together. Toughness d 0.01 E d + K n d E K 0.75 (n 1) (n 1) N/m 2 2 (0.01) N/m 2 ( ) (0.75) 1.3 (0.01) J/m 3 ( in.-lb f /in. 3 ) Question 6.49: A cylindrical specimen of a brass alloy 7.5 mm (0.30 in.) in diameter and 90.0 mm (3.54 in.) long is pulled in tension with a force of 6000 N (1350 lb f ); the force is subsequently released.
15 (a) Compute the final length of the specimen at this time. The tensile stress strain behavior for this alloy is shown in Figure (b) Compute the final specimen length when the load is increased to 16,500 N (3700 lb f ) and then released. (a) In order to determine the final length of the brass specimen when the load is released, it first becomes necessary to compute the applied stress using Equation 6.1; thus F A 0 F d N m MPa (19,000 psi) Upon locating this point on the stress-strain curve (Figure 6.12), we note that it is in the linear, elastic region; therefore, when the load is released the specimen will return to its original length of 90 mm (3.54 in.). (b) In this portion of the problem we are asked to calculate the final length, after load release, when the load is increased to 16,500 N (3700 lb f ). Again, computing the stress 16,500 N m MPa (52,300 psi) The point on the stress-strain curve corresponding to this stress is in the plastic region. We are able to estimate the amount of permanent strain by drawing a straight line parallel to the linear elastic region; this line intersects the strain axis at a strain of about 0.08 which is the amount of plastic strain. The final specimen length l i may be determined from a rearranged form of Equation 6.2 as l i l 0 (1 + ) (90 mm)( ) mm (3.82 in.) Question 6.D1: A large tower is to be supported by a series of steel wires. It is estimated that the load on each wire will be 11,100 N (2500 lb f ). Determine the minimum required wire diameter assuming a factor of safety of 2 and a yield strength of 1030 MPa (150,000 psi).
16 For this problem the working stress is computed using Equation 6.24 with N 2, as w y MPa MPa (75,000 psi ) Since the force is given, the area may be determined from Equation 6.1, and subsequently the original diameter d 0 may be calculated as A 0 F d 2 0 w 2 And d 0 4F w (4)(11,100 N) ( N/m 2 ) m 5.23 mm (0.206 in.) Question 6.D2: (a) Gaseous hydrogen at a constant pressure of MPa (10 atm) is to flow within the inside of a thin-walled cylindrical tube of nickel that has a radius of 0.1 m. The temperature of the tube is to be 300 C and the pressure of hydrogen outside of the tube will be maintained at MPa (0.1 atm). Calculate the minimum wall thickness if the diffusion flux is to be no greater than mol/m 2 -s. The concentration of hydrogen in the nickel, C H (in moles hydrogen per m 3 of Ni) is a function of hydrogen pressure, P H2 (in MPa) and absolute temperature (T) according to 12.3 kj/mol C H 30.8 p H2 exp (6.28) RT Furthermore, the diffusion coefficient for the diffusion of H in Ni depends on temperature as D H exp kj/mol RT (6.29)
17 (b) For thin-walled cylindrical tubes that are pressurized, the circumferential stress is a function of the pressure difference across the wall (Δp), cylinder radius (r), and tube thickness (Δx) as r p 4 x (6.30) Compute the circumferential stress to which the walls of this pressurized cylinder are exposed. (c) The room-temperature yield strength of Ni is 100 MPa (15,000 psi) and, furthermore, s y diminishes about 5 MPa for every 50 C rise in temperature. Would you expect the wall thickness computed in part (b) to be suitable for this Ni cylinder at 300 C? Why or why not? (d) If this thickness is found to be suitable, compute the minimum thickness that could be used without any deformation of the tube walls. How much would the diffusion flux increase with this reduction in thickness? On the other hand, if the thickness determined in part (c) is found to be unsuitable, then specify a minimum thickness that you would use. In this case, how much of a diminishment in diffusion flux would result? (a) This portion of the problem asks for us to compute the wall thickness of a thin-walled cylindrical Ni tube at 300 C through which hydrogen gas diffuses. The inside and outside pressures are, respectively, and MPa, and the diffusion flux is to be no greater than mol/m 2 -s. This is a steady-state diffusion problem, which necessitates that we employ Equation 5.3. The concentrations at the inside and outside wall faces may be determined using Equation 6.28, and, furthermore, the diffusion coefficient is computed using Equation Solving for x (using Equation 5.3) x D C J mol/m 2 s ( ,560 J /mol ) exp (8.31 J/mol- K)( K) 12, 300 J/mol (30.8) exp MPa MPa (8.31 J/mol- K)( K)
18 m 2.5 mm (b) Now we are asked to determine the circumferential stress: r p 4 x (0.10 m)(1.013 MPa MPa) (4)( m) 10.0 MPa (c) Now we are to compare this value of stress to the yield strength of Ni at 300 C, from which it is possible to determine whether or not the 2.5 mm wall thickness is suitable. From the information given in the problem, we may write an equation for the dependence of yield strength ( y ) on temperature (T) as follows: y 100 MPa 5 MPa 50 C T T r where T r is room temperature and for temperature in degrees Celsius. Thus, at 300 C y 100 MPa (0.1 MPa/ C) (300 C 20 C) 72 MPa Inasmuch as the circumferential stress (10 MPa) is much less than the yield strength (72 MPa), this thickness is entirely suitable. (d) And, finally, this part of the problem asks that we specify how much this thickness may be reduced and still retain a safe design. Let us use a working stress by dividing the yield stress by a factor of safety, according to Equation On the basis of our experience, let us use a value of 2.0 for N. Thus w y N 72 MPa 2 36 MPa Using this value for w and Equation 6.30, we now compute the tube thickness as
19 x r p 4 w (0.10 m)(1.013 MPa MPa) 4(36 MPa) m 0.70 mm Substitution of this value into Fick's first law we calculate the diffusion flux as follows: J D C x ( , 560 J/mol ) exp (8.31 J/mol- K)( K) 12,300 J /mol (30.8) exp (8.31 J/mol- K)( K) MPa MPa m mol/m 2 -s Thus, the flux increases by approximately a factor of 3.5, from to mol/m 2 -s with this reduction in thickness.